# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Eu3Sn2P4_Cmca
_database_code_depnum_ccdc_archive 'CCDC 1915387'
loop_
_audit_author_name
_audit_author_address
'Weiwei Xie'
;Louisiana State University 
United States of America
;
_audit_update_record             
;
2019-05-10 deposited with the CCDC.	2019-09-10 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2013
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Eu3 P4 Sn2'
_chemical_formula_weight         817.14

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           64
_space_group_name_H-M_alt        'C m c a'
_space_group_name_Hall           '-C 2bc 2'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1, z+1/2'
'-x+1/2, y+1, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y-1/2, -z-1/2'
'x, -y-1/2, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y, -z-1/2'
'x+1/2, -y, z-1/2'
'-x+1/2, y+1/2, z'

_cell_length_a                   24.882(3)
_cell_length_b                   12.4534(17)
_cell_length_c                   18.493(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     5730.4(13)
_cell_formula_units_Z            24
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    6427
_cell_measurement_theta_min      1.637
_cell_measurement_theta_max      35.128

_exptl_crystal_description       crystasize_0.5_0.5_0.5
_exptl_crystal_colour            Metallic
_exptl_crystal_density_meas      None
_exptl_crystal_density_method    'Not measured'
_exptl_crystal_density_diffrn    5.683
_exptl_crystal_F_000             8376
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.030
_exptl_crystal_size_mid          0.020
_exptl_crystal_size_min          0.015
_exptl_absorpt_coefficient_mu    25.154
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   Numerical
_exptl_absorpt_correction_T_min  0.3724
_exptl_absorpt_correction_T_max  0.7463
_exptl_absorpt_process_details   'SADABS Sheldrick'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  Kappa_Apex_II_Bruker_KaptonLoop
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            34498
_diffrn_reflns_av_unetI/netI     0.0542
_diffrn_reflns_av_R_equivalents  0.0725
_diffrn_reflns_limit_h_min       -40
_diffrn_reflns_limit_h_max       40
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         1.637
_diffrn_reflns_theta_max         35.128
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.990
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.990
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             6427
_reflns_number_gt                4564
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0062P)²+29.8076P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    None
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.0000157(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         6427
_refine_ls_number_parameters     132
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0668
_refine_ls_R_factor_gt           0.0354
_refine_ls_wR_factor_ref         0.0578
_refine_ls_wR_factor_gt          0.0494
_refine_ls_goodness_of_fit_ref   1.029
_refine_ls_restrained_S_all      1.029
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Eu1 Eu 0.5000 0.0000 0.5000 0.00925(11) Uani 1 4 d S T P . .
Eu2 Eu 0.41655(2) 0.21167(3) 0.36854(2) 0.00996(6) Uani 1 1 d . . . . .
Eu3 Eu 0.32474(2) 0.0000 0.5000 0.01058(8) Uani 1 2 d S T P . .
Eu4 Eu 0.5000 0.06195(4) 0.72913(2) 0.01119(9) Uani 1 2 d S T P . .
Eu5 Eu 0.33136(2) 0.45203(3) 0.24108(2) 0.01023(6) Uani 1 1 d . . . . .
Eu6 Eu 0.5000 0.5000 0.5000 0.01552(13) Uani 1 4 d S T P . .
Eu7 Eu 0.24451(2) 0.21136(3) 0.37253(2) 0.01214(6) Uani 1 1 d . . . . .
Sn1 Sn 0.41768(2) 0.20852(3) 0.56480(2) 0.00874(8) Uani 1 1 d . . . . .
Sn2 Sn 0.33764(2) 0.43430(3) 0.43911(2) 0.00875(8) Uani 1 1 d . . . . .
Sn3 Sn 0.41464(2) 0.15057(3) 0.17902(2) 0.00883(8) Uani 1 1 d . . . . .
P1 P 0.5000 0.24971(19) 0.48636(12) 0.0096(4) Uani 1 2 d S T P . .
P2 P 0.33463(6) 0.20128(13) 0.25263(9) 0.0100(3) Uani 1 1 d . . . . .
P3 P 0.41309(7) 0.02539(12) 0.61603(8) 0.0099(3) Uani 1 1 d . . . . .
P4 P 0.5000 0.18685(19) 0.25214(13) 0.0100(4) Uani 1 2 d S T P . .
P5 P 0.42318(6) 0.45738(14) 0.36393(9) 0.0107(3) Uani 1 1 d . . . . .
P6 P 0.24663(6) 0.03885(14) 0.62761(9) 0.0104(3) Uani 1 1 d . . . . .
P7 P 0.33348(6) 0.24424(13) 0.48996(9) 0.0099(3) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Eu1 P3 3.0627(16) 12_655 ?
Eu1 P3 3.0627(16) 4_556 ?
Eu1 P3 3.0627(16) 9_656 ?
Eu1 P3 3.0627(16) . ?
Eu1 P1 3.120(2) 9_656 ?
Eu1 P1 3.120(2) . ?
Eu1 Sn1 3.5178(5) 12_655 ?
Eu1 Sn1 3.5178(5) 4_556 ?
Eu1 Sn1 3.5178(5) 9_656 ?
Eu1 Sn1 3.5178(5) . ?
Eu1 Eu2 4.1437(4) 9_656 ?
Eu1 Eu2 4.1437(4) 4_556 ?
Eu2 P2 2.9608(17) . ?
Eu2 P3 2.9672(16) 4_556 ?
Eu2 P4 3.0068(17) . ?
Eu2 P1 3.0469(17) . ?
Eu2 P5 3.0656(18) . ?
Eu2 P7 3.0787(17) . ?
Eu2 Sn3 3.5867(7) . ?
Eu2 Sn1 3.6297(7) . ?
Eu2 Sn2 3.6393(6) . ?
Eu2 Eu2 4.1529(8) 12_655 ?
Eu2 Eu3 4.2517(5) . ?
Eu3 P7 3.0551(16) . ?
Eu3 P7 3.0551(16) 4_556 ?
Eu3 P3 3.0882(17) 4_556 ?
Eu3 P3 3.0882(17) . ?
Eu3 P6 3.0953(17) 4_556 ?
Eu3 P6 3.0953(17) . ?
Eu3 Sn1 3.6779(6) 4_556 ?
Eu3 Sn1 3.6779(6) . ?
Eu3 Eu7 4.0584(5) 4_556 ?
Eu3 Eu7 4.0584(5) . ?
Eu3 Eu2 4.2517(5) 4_556 ?
Eu4 P3 3.0427(17) . ?
Eu4 P3 3.0427(17) 12_655 ?
Eu4 P4 3.118(2) 9_656 ?
Eu4 P5 3.1505(16) 2_655 ?
Eu4 P5 3.1505(16) 11_566 ?
Eu4 P4 3.157(2) 2_655 ?
Eu4 Sn3 3.7950(6) 4_556 ?
Eu4 Sn3 3.7950(6) 9_656 ?
Eu4 Eu5 4.2056(6) 2_655 ?
Eu4 Eu5 4.2056(6) 11_566 ?
Eu4 Eu2 4.3481(6) 2_655 ?
Eu5 P6 2.9768(16) 11_565 ?
Eu5 P3 3.0925(16) 11_565 ?
Eu5 P2 3.1073(17) 10_566 ?
Eu5 P6 3.1105(17) 13_556 ?
Eu5 P2 3.1310(17) . ?
Eu5 P5 3.2227(17) . ?
Eu5 Sn3 3.5483(6) 10_566 ?
Eu5 Sn2 3.6720(7) . ?
Eu5 Eu5 4.0623(8) 7_545 ?
Eu5 Eu7 4.1184(6) 7_545 ?
Eu5 Eu4 4.2056(6) 2_654 ?
Eu6 P1 3.127(2) . ?
Eu6 P1 3.127(2) 9_666 ?
Eu6 P5 3.2042(17) . ?
Eu6 P5 3.2043(17) 9_666 ?
Eu6 P5 3.2043(17) 12_655 ?
Eu6 P5 3.2043(17) 4_566 ?
Eu7 P2 3.0415(17) 7_545 ?
Eu7 P6 3.1164(18) 4_556 ?
Eu7 P6 3.1186(18) 13_556 ?
Eu7 P7 3.1280(16) . ?
Eu7 P2 3.1561(17) . ?
Eu7 P7 3.2461(17) 13_556 ?
Eu7 Sn2 3.8203(6) . ?
Eu7 Eu5 4.1183(6) 7_545 ?
Eu7 Eu5 4.4176(6) 10_556 ?
Sn1 P3 2.4722(16) . ?
Sn1 P7 2.5500(16) . ?
Sn1 P1 2.5618(14) . ?
Sn1 Sn3 2.7471(6) 11_566 ?
Sn2 P6 2.4558(16) 13_556 ?
Sn2 P7 2.5489(16) . ?
Sn2 P5 2.5584(16) . ?
Sn2 Sn2 2.7838(9) 4_566 ?
Sn3 P2 2.4931(17) . ?
Sn3 P5 2.5425(17) 10_556 ?
Sn3 P4 2.5581(14) . ?
Sn3 Sn1 2.7472(6) 11_565 ?
Sn3 Eu5 3.5483(6) 10_556 ?
Sn3 Eu4 3.7949(6) 9_656 ?
P1 Sn1 2.5618(14) 12_655 ?
P1 Eu2 3.0469(17) 12_655 ?
P2 Eu7 3.0415(17) 7_545 ?
P2 Eu5 3.1073(17) 10_556 ?
P3 Eu2 2.9673(16) 4_556 ?
P3 Eu5 3.0924(16) 11_566 ?
P4 Sn3 2.5582(14) 12_655 ?
P4 Eu2 3.0068(17) 12_655 ?
P4 Eu4 3.118(2) 9_656 ?
P4 Eu4 3.157(2) 2_654 ?
P5 Sn3 2.5425(17) 10_566 ?
P5 Eu4 3.1505(16) 2_654 ?
P6 Sn2 2.4558(16) 13_556 ?
P6 Eu5 2.9768(16) 11_566 ?
P6 Eu5 3.1105(17) 13_556 ?
P6 Eu7 3.1164(18) 4_556 ?
P6 Eu7 3.1186(18) 13_556 ?
P7 Eu7 3.2462(17) 13_556 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
P3 Eu1 P3 180.00(4) 12_655 4_556 ?
P3 Eu1 P3 90.17(6) 12_655 9_656 ?
P3 Eu1 P3 89.83(6) 4_556 9_656 ?
P3 Eu1 P3 89.83(6) 12_655 . ?
P3 Eu1 P3 90.17(6) 4_556 . ?
P3 Eu1 P3 180.0 9_656 . ?
P3 Eu1 P1 92.65(4) 12_655 9_656 ?
P3 Eu1 P1 87.35(4) 4_556 9_656 ?
P3 Eu1 P1 87.35(4) 9_656 9_656 ?
P3 Eu1 P1 92.65(4) . 9_656 ?
P3 Eu1 P1 87.35(4) 12_655 . ?
P3 Eu1 P1 92.65(4) 4_556 . ?
P3 Eu1 P1 92.65(4) 9_656 . ?
P3 Eu1 P1 87.35(4) . . ?
P1 Eu1 P1 180.0 9_656 . ?
P3 Eu1 Sn1 43.45(3) 12_655 12_655 ?
P3 Eu1 Sn1 136.55(3) 4_556 12_655 ?
P3 Eu1 Sn1 84.48(3) 9_656 12_655 ?
P3 Eu1 Sn1 95.52(3) . 12_655 ?
P1 Eu1 Sn1 135.09(3) 9_656 12_655 ?
P1 Eu1 Sn1 44.91(3) . 12_655 ?
P3 Eu1 Sn1 136.55(3) 12_655 4_556 ?
P3 Eu1 Sn1 43.45(3) 4_556 4_556 ?
P3 Eu1 Sn1 95.52(3) 9_656 4_556 ?
P3 Eu1 Sn1 84.48(3) . 4_556 ?
P1 Eu1 Sn1 44.91(3) 9_656 4_556 ?
P1 Eu1 Sn1 135.09(3) . 4_556 ?
Sn1 Eu1 Sn1 180.0 12_655 4_556 ?
P3 Eu1 Sn1 84.48(3) 12_655 9_656 ?
P3 Eu1 Sn1 95.52(3) 4_556 9_656 ?
P3 Eu1 Sn1 43.45(3) 9_656 9_656 ?
P3 Eu1 Sn1 136.55(3) . 9_656 ?
P1 Eu1 Sn1 44.91(2) 9_656 9_656 ?
P1 Eu1 Sn1 135.09(3) . 9_656 ?
Sn1 Eu1 Sn1 108.777(16) 12_655 9_656 ?
Sn1 Eu1 Sn1 71.223(16) 4_556 9_656 ?
P3 Eu1 Sn1 95.52(3) 12_655 . ?
P3 Eu1 Sn1 84.48(3) 4_556 . ?
P3 Eu1 Sn1 136.55(3) 9_656 . ?
P3 Eu1 Sn1 43.45(3) . . ?
P1 Eu1 Sn1 135.09(3) 9_656 . ?
P1 Eu1 Sn1 44.91(3) . . ?
Sn1 Eu1 Sn1 71.222(16) 12_655 . ?
Sn1 Eu1 Sn1 108.778(16) 4_556 . ?
Sn1 Eu1 Sn1 180.0 9_656 . ?
P3 Eu1 Eu2 45.64(3) 12_655 9_656 ?
P3 Eu1 Eu2 134.36(3) 4_556 9_656 ?
P3 Eu1 Eu2 89.52(3) 9_656 9_656 ?
P3 Eu1 Eu2 90.48(3) . 9_656 ?
P1 Eu1 Eu2 47.04(3) 9_656 9_656 ?
P1 Eu1 Eu2 132.96(3) . 9_656 ?
Sn1 Eu1 Eu2 88.737(12) 12_655 9_656 ?
Sn1 Eu1 Eu2 91.263(12) 4_556 9_656 ?
Sn1 Eu1 Eu2 55.839(11) 9_656 9_656 ?
Sn1 Eu1 Eu2 124.161(10) . 9_656 ?
P3 Eu1 Eu2 90.48(3) 12_655 4_556 ?
P3 Eu1 Eu2 89.52(3) 4_556 4_556 ?
P3 Eu1 Eu2 134.36(3) 9_656 4_556 ?
P3 Eu1 Eu2 45.64(3) . 4_556 ?
P1 Eu1 Eu2 47.04(3) 9_656 4_556 ?
P1 Eu1 Eu2 132.96(3) . 4_556 ?
Sn1 Eu1 Eu2 124.161(11) 12_655 4_556 ?
Sn1 Eu1 Eu2 55.839(11) 4_556 4_556 ?
Sn1 Eu1 Eu2 91.263(12) 9_656 4_556 ?
Sn1 Eu1 Eu2 88.737(12) . 4_556 ?
Eu2 Eu1 Eu2 60.146(12) 9_656 4_556 ?
P2 Eu2 P3 90.35(4) . 4_556 ?
P2 Eu2 P4 87.29(5) . . ?
P3 Eu2 P4 89.23(6) 4_556 . ?
P2 Eu2 P1 173.56(6) . . ?
P3 Eu2 P1 96.06(5) 4_556 . ?
P4 Eu2 P1 93.28(4) . . ?
P2 Eu2 P5 93.47(4) . . ?
P3 Eu2 P5 175.83(4) 4_556 . ?
P4 Eu2 P5 92.61(5) . . ?
P1 Eu2 P5 80.10(5) . . ?
P2 Eu2 P7 94.10(4) . . ?
P3 Eu2 P7 92.38(4) 4_556 . ?
P4 Eu2 P7 177.86(5) . . ?
P1 Eu2 P7 85.15(4) . . ?
P5 Eu2 P7 85.69(4) . . ?
P2 Eu2 Sn3 43.46(3) . . ?
P3 Eu2 Sn3 83.25(3) 4_556 . ?
P4 Eu2 Sn3 44.59(3) . . ?
P1 Eu2 Sn3 137.80(3) . . ?
P5 Eu2 Sn3 100.68(3) . . ?
P7 Eu2 Sn3 137.03(3) . . ?
P2 Eu2 Sn1 136.78(3) . . ?
P3 Eu2 Sn1 83.87(3) 4_556 . ?
P4 Eu2 Sn1 135.18(3) . . ?
P1 Eu2 Sn1 44.06(3) . . ?
P5 Eu2 Sn1 92.19(3) . . ?
P7 Eu2 Sn1 43.73(3) . . ?
Sn3 Eu2 Sn1 167.129(14) . . ?
P2 Eu2 Sn2 85.50(3) . . ?
P3 Eu2 Sn2 135.06(3) 4_556 . ?
P4 Eu2 Sn2 135.04(5) . . ?
P1 Eu2 Sn2 89.59(4) . . ?
P5 Eu2 Sn2 43.83(3) . . ?
P7 Eu2 Sn2 43.61(3) . . ?
Sn3 Eu2 Sn2 120.322(12) . . ?
Sn1 Eu2 Sn2 69.749(11) . . ?
P2 Eu2 Eu1 137.90(3) . . ?
P3 Eu2 Eu1 47.56(3) 4_556 . ?
P4 Eu2 Eu1 90.49(4) . . ?
P1 Eu2 Eu1 48.54(4) . . ?
P5 Eu2 Eu1 128.63(3) . . ?
P7 Eu2 Eu1 89.56(3) . . ?
Sn3 Eu2 Eu1 116.422(12) . . ?
Sn1 Eu2 Eu1 53.316(9) . . ?
Sn2 Eu2 Eu1 122.997(13) . . ?
P2 Eu2 Eu2 133.51(3) . 12_655 ?
P3 Eu2 Eu2 91.66(3) 4_556 12_655 ?
P4 Eu2 Eu2 46.32(3) . 12_655 ?
P1 Eu2 Eu2 47.04(3) . 12_655 ?
P5 Eu2 Eu2 86.91(3) . 12_655 ?
P7 Eu2 Eu2 132.17(3) . 12_655 ?
Sn3 Eu2 Eu2 90.759(8) . 12_655 ?
Sn1 Eu2 Eu2 89.556(8) . 12_655 ?
Sn2 Eu2 Eu2 122.649(9) . 12_655 ?
Eu1 Eu2 Eu2 59.926(6) . 12_655 ?
P2 Eu2 Eu3 90.97(3) . . ?
P3 Eu2 Eu3 46.57(3) 4_556 . ?
P4 Eu2 Eu3 135.78(5) . . ?
P1 Eu2 Eu3 93.08(4) . . ?
P5 Eu2 Eu3 131.58(3) . . ?
P7 Eu2 Eu3 45.89(3) . . ?
Sn3 Eu2 Eu3 114.840(12) . . ?
Sn1 Eu2 Eu3 54.951(9) . . ?
Sn2 Eu2 Eu3 88.707(13) . . ?
Eu1 Eu2 Eu3 62.572(11) . . ?
Eu2 Eu2 Eu3 122.498(7) 12_655 . ?
P7 Eu3 P7 171.84(6) . 4_556 ?
P7 Eu3 P3 90.52(4) . 4_556 ?
P7 Eu3 P3 83.66(4) 4_556 4_556 ?
P7 Eu3 P3 83.66(4) . . ?
P7 Eu3 P3 90.52(4) 4_556 . ?
P3 Eu3 P3 89.23(6) 4_556 . ?
P7 Eu3 P6 98.86(4) . 4_556 ?
P7 Eu3 P6 86.30(5) 4_556 4_556 ?
P3 Eu3 P6 84.33(4) 4_556 4_556 ?
P3 Eu3 P6 173.09(4) . 4_556 ?
P7 Eu3 P6 86.30(5) . . ?
P7 Eu3 P6 98.86(4) 4_556 . ?
P3 Eu3 P6 173.09(4) 4_556 . ?
P3 Eu3 P6 84.33(4) . . ?
P6 Eu3 P6 102.20(6) 4_556 . ?
P7 Eu3 Sn1 129.67(3) . 4_556 ?
P7 Eu3 Sn1 43.29(3) 4_556 4_556 ?
P3 Eu3 Sn1 41.73(3) 4_556 4_556 ?
P3 Eu3 Sn1 81.44(3) . 4_556 ?
P6 Eu3 Sn1 92.07(3) 4_556 4_556 ?
P6 Eu3 Sn1 138.90(3) . 4_556 ?
P7 Eu3 Sn1 43.29(3) . . ?
P7 Eu3 Sn1 129.67(3) 4_556 . ?
P3 Eu3 Sn1 81.44(3) 4_556 . ?
P3 Eu3 Sn1 41.73(3) . . ?
P6 Eu3 Sn1 138.90(3) 4_556 . ?
P6 Eu3 Sn1 92.07(3) . . ?
Sn1 Eu3 Sn1 102.083(19) 4_556 . ?
P7 Eu3 Eu7 135.73(3) . 4_556 ?
P7 Eu3 Eu7 49.76(3) 4_556 4_556 ?
P3 Eu3 Eu7 133.42(3) 4_556 4_556 ?
P3 Eu3 Eu7 90.75(3) . 4_556 ?
P6 Eu3 Eu7 91.86(3) 4_556 4_556 ?
P6 Eu3 Eu7 49.43(3) . 4_556 ?
Sn1 Eu3 Eu7 92.328(12) 4_556 4_556 ?
Sn1 Eu3 Eu7 125.309(11) . 4_556 ?
P7 Eu3 Eu7 49.76(3) . . ?
P7 Eu3 Eu7 135.73(3) 4_556 . ?
P3 Eu3 Eu7 90.75(3) 4_556 . ?
P3 Eu3 Eu7 133.42(3) . . ?
P6 Eu3 Eu7 49.43(3) 4_556 . ?
P6 Eu3 Eu7 91.86(3) . . ?
Sn1 Eu3 Eu7 125.310(10) 4_556 . ?
Sn1 Eu3 Eu7 92.328(12) . . ?
Eu7 Eu3 Eu7 121.064(16) 4_556 . ?
P7 Eu3 Eu2 46.35(3) . . ?
P7 Eu3 Eu2 127.86(3) 4_556 . ?
P3 Eu3 Eu2 44.25(3) 4_556 . ?
P3 Eu3 Eu2 87.21(3) . . ?
P6 Eu3 Eu2 89.91(3) 4_556 . ?
P6 Eu3 Eu2 132.56(3) . . ?
Sn1 Eu3 Eu2 85.046(14) 4_556 . ?
Sn1 Eu3 Eu2 53.895(11) . . ?
Eu7 Eu3 Eu2 176.886(12) 4_556 . ?
Eu7 Eu3 Eu2 61.971(10) . . ?
P7 Eu3 Eu2 127.86(3) . 4_556 ?
P7 Eu3 Eu2 46.35(3) 4_556 4_556 ?
P3 Eu3 Eu2 87.21(3) 4_556 4_556 ?
P3 Eu3 Eu2 44.25(3) . 4_556 ?
P6 Eu3 Eu2 132.56(3) 4_556 4_556 ?
P6 Eu3 Eu2 89.91(3) . 4_556 ?
Sn1 Eu3 Eu2 53.895(11) 4_556 4_556 ?
Sn1 Eu3 Eu2 85.045(13) . 4_556 ?
Eu7 Eu3 Eu2 61.972(10) 4_556 4_556 ?
Eu7 Eu3 Eu2 176.885(12) . 4_556 ?
Eu2 Eu3 Eu2 115.003(15) . 4_556 ?
P3 Eu4 P3 90.58(6) . 12_655 ?
P3 Eu4 P4 85.85(4) . 9_656 ?
P3 Eu4 P4 85.85(4) 12_655 9_656 ?
P3 Eu4 P5 164.51(5) . 2_655 ?
P3 Eu4 P5 95.81(4) 12_655 2_655 ?
P4 Eu4 P5 80.57(5) 9_656 2_655 ?
P3 Eu4 P5 95.81(4) . 11_566 ?
P3 Eu4 P5 164.51(5) 12_655 11_566 ?
P4 Eu4 P5 80.57(5) 9_656 11_566 ?
P5 Eu4 P5 74.70(6) 2_655 11_566 ?
P3 Eu4 P4 103.94(4) . 2_655 ?
P3 Eu4 P4 103.94(4) 12_655 2_655 ?
P4 Eu4 P4 165.876(16) 9_656 2_655 ?
P5 Eu4 P4 88.23(5) 2_655 2_655 ?
P5 Eu4 P4 88.23(5) 11_566 2_655 ?
P3 Eu4 Sn3 78.79(3) . 4_556 ?
P3 Eu4 Sn3 126.95(3) 12_655 4_556 ?
P4 Eu4 Sn3 42.03(3) 9_656 4_556 ?
P5 Eu4 Sn3 86.11(3) 2_655 4_556 ?
P5 Eu4 Sn3 41.67(3) 11_566 4_556 ?
P4 Eu4 Sn3 129.10(3) 2_655 4_556 ?
P3 Eu4 Sn3 126.95(3) . 9_656 ?
P3 Eu4 Sn3 78.79(3) 12_655 9_656 ?
P4 Eu4 Sn3 42.03(2) 9_656 9_656 ?
P5 Eu4 Sn3 41.67(3) 2_655 9_656 ?
P5 Eu4 Sn3 86.11(3) 11_566 9_656 ?
P4 Eu4 Sn3 129.10(3) 2_655 9_656 ?
Sn3 Eu4 Sn3 68.072(17) 4_556 9_656 ?
P3 Eu4 Eu5 137.65(3) . 2_655 ?
P3 Eu4 Eu5 47.22(3) 12_655 2_655 ?
P4 Eu4 Eu5 87.308(8) 9_656 2_655 ?
P5 Eu4 Eu5 49.45(3) 2_655 2_655 ?
P5 Eu4 Eu5 124.10(3) 11_566 2_655 ?
P4 Eu4 Eu5 91.944(8) 2_655 2_655 ?
Sn3 Eu4 Eu5 120.403(13) 4_556 2_655 ?
Sn3 Eu4 Eu5 52.350(9) 9_656 2_655 ?
P3 Eu4 Eu5 47.22(3) . 11_566 ?
P3 Eu4 Eu5 137.65(3) 12_655 11_566 ?
P4 Eu4 Eu5 87.308(8) 9_656 11_566 ?
P5 Eu4 Eu5 124.10(3) 2_655 11_566 ?
P5 Eu4 Eu5 49.45(3) 11_566 11_566 ?
P4 Eu4 Eu5 91.944(8) 2_655 11_566 ?
Sn3 Eu4 Eu5 52.350(9) 4_556 11_566 ?
Sn3 Eu4 Eu5 120.403(13) 9_656 11_566 ?
Eu5 Eu4 Eu5 172.330(15) 2_655 11_566 ?
P3 Eu4 Eu1 45.32(3) . . ?
P3 Eu4 Eu1 45.32(3) 12_655 . ?
P4 Eu4 Eu1 86.06(4) 9_656 . ?
P5 Eu4 Eu1 139.89(3) 2_655 . ?
P5 Eu4 Eu1 139.89(3) 11_566 . ?
P4 Eu4 Eu1 108.06(4) 2_655 . ?
Sn3 Eu4 Eu1 108.388(12) 4_556 . ?
Sn3 Eu4 Eu1 108.388(12) 9_656 . ?
Eu5 Eu4 Eu1 92.538(7) 2_655 . ?
Eu5 Eu4 Eu1 92.538(7) 11_566 . ?
P3 Eu4 Eu2 147.56(3) . 2_655 ?
P3 Eu4 Eu2 99.51(3) 12_655 2_655 ?
P4 Eu4 Eu2 125.34(4) 9_656 2_655 ?
P5 Eu4 Eu2 44.82(3) 2_655 2_655 ?
P5 Eu4 Eu2 82.54(3) 11_566 2_655 ?
P4 Eu4 Eu2 43.75(3) 2_655 2_655 ?
Sn3 Eu4 Eu2 117.006(16) 4_556 2_655 ?
Sn3 Eu4 Eu2 85.383(14) 9_656 2_655 ?
Eu5 Eu4 Eu2 61.262(8) 2_655 2_655 ?
Eu5 Eu4 Eu2 118.174(12) 11_566 2_655 ?
Eu1 Eu4 Eu2 134.384(10) . 2_655 ?
P6 Eu5 P3 86.28(5) 11_565 11_565 ?
P6 Eu5 P2 90.39(5) 11_565 10_566 ?
P3 Eu5 P2 85.41(4) 11_565 10_566 ?
P6 Eu5 P6 96.15(4) 11_565 13_556 ?
P3 Eu5 P6 172.21(4) 11_565 13_556 ?
P2 Eu5 P6 87.17(4) 10_566 13_556 ?
P6 Eu5 P2 96.00(5) 11_565 . ?
P3 Eu5 P2 97.16(4) 11_565 . ?
P2 Eu5 P2 173.25(3) 10_566 . ?
P6 Eu5 P2 89.96(4) 13_556 . ?
P6 Eu5 P5 176.63(4) 11_565 . ?
P3 Eu5 P5 93.39(4) 11_565 . ?
P2 Eu5 P5 86.24(4) 10_566 . ?
P6 Eu5 P5 83.75(4) 13_556 . ?
P2 Eu5 P5 87.37(4) . . ?
P6 Eu5 Sn3 132.89(4) 11_565 10_566 ?
P3 Eu5 Sn3 82.18(3) 11_565 10_566 ?
P2 Eu5 Sn3 43.37(3) 10_566 10_566 ?
P6 Eu5 Sn3 90.79(3) 13_556 10_566 ?
P2 Eu5 Sn3 130.65(3) . 10_566 ?
P5 Eu5 Sn3 43.78(3) . 10_566 ?
P6 Eu5 Sn2 137.35(3) 11_565 . ?
P3 Eu5 Sn2 136.32(3) 11_565 . ?
P2 Eu5 Sn2 91.24(3) 10_566 . ?
P6 Eu5 Sn2 41.43(3) 13_556 . ?
P2 Eu5 Sn2 82.58(3) . . ?
P5 Eu5 Sn2 42.95(3) . . ?
Sn3 Eu5 Sn2 66.530(11) 10_566 . ?
P6 Eu5 Eu5 49.56(3) 11_565 7_545 ?
P3 Eu5 Eu5 135.74(3) 11_565 7_545 ?
P2 Eu5 Eu5 91.32(3) 10_566 7_545 ?
P6 Eu5 Eu5 46.75(3) 13_556 7_545 ?
P2 Eu5 Eu5 91.16(3) . 7_545 ?
P5 Eu5 Eu5 130.49(3) . 7_545 ?
Sn3 Eu5 Eu5 123.245(12) 10_566 7_545 ?
Sn2 Eu5 Eu5 87.791(12) . 7_545 ?
P6 Eu5 Eu7 48.97(3) 11_565 7_545 ?
P3 Eu5 Eu7 89.20(3) 11_565 7_545 ?
P2 Eu5 Eu7 139.29(3) 10_566 7_545 ?
P6 Eu5 Eu7 97.98(3) 13_556 7_545 ?
P2 Eu5 Eu7 47.23(3) . 7_545 ?
P5 Eu5 Eu7 134.40(3) . 7_545 ?
Sn3 Eu5 Eu7 170.838(12) 10_566 7_545 ?
Sn2 Eu5 Eu7 118.984(12) . 7_545 ?
Eu5 Eu5 Eu7 65.454(8) 7_545 7_545 ?
P6 Eu5 Eu4 132.16(3) 11_565 2_654 ?
P3 Eu5 Eu4 46.24(3) 11_565 2_654 ?
P2 Eu5 Eu4 90.99(3) 10_566 2_654 ?
P6 Eu5 Eu4 131.68(3) 13_556 2_654 ?
P2 Eu5 Eu4 86.35(3) . 2_654 ?
P5 Eu5 Eu4 47.97(3) . 2_654 ?
Sn3 Eu5 Eu4 57.864(11) 10_566 2_654 ?
Sn2 Eu5 Eu4 90.425(11) . 2_654 ?
Eu5 Eu5 Eu4 177.115(10) 7_545 2_654 ?
Eu7 Eu5 Eu4 113.604(11) 7_545 2_654 ?
P6 Eu5 Eu2 138.73(3) 11_565 . ?
P3 Eu5 Eu2 98.45(3) 11_565 . ?
P2 Eu5 Eu2 130.76(3) 10_566 . ?
P6 Eu5 Eu2 84.63(3) 13_556 . ?
P2 Eu5 Eu2 42.76(3) . . ?
P5 Eu5 Eu2 44.64(3) . . ?
Sn3 Eu5 Eu2 88.244(14) 10_566 . ?
Sn2 Eu5 Eu2 53.049(9) . . ?
Eu5 Eu5 Eu2 116.147(10) 7_545 . ?
Eu7 Eu5 Eu2 89.945(13) 7_545 . ?
Eu4 Eu5 Eu2 60.981(9) 2_654 . ?
P1 Eu6 P1 180.0 . 9_666 ?
P1 Eu6 P5 76.80(4) . . ?
P1 Eu6 P5 103.20(4) 9_666 . ?
P1 Eu6 P5 103.20(4) . 9_666 ?
P1 Eu6 P5 76.80(4) 9_666 9_666 ?
P5 Eu6 P5 180.00(6) . 9_666 ?
P1 Eu6 P5 76.80(4) . 12_655 ?
P1 Eu6 P5 103.20(4) 9_666 12_655 ?
P5 Eu6 P5 73.24(6) . 12_655 ?
P5 Eu6 P5 106.76(6) 9_666 12_655 ?
P1 Eu6 P5 103.20(4) . 4_566 ?
P1 Eu6 P5 76.80(4) 9_666 4_566 ?
P5 Eu6 P5 106.76(6) . 4_566 ?
P5 Eu6 P5 73.24(6) 9_666 4_566 ?
P5 Eu6 P5 180.0 12_655 4_566 ?
P2 Eu7 P6 88.23(4) 7_545 4_556 ?
P2 Eu7 P6 94.95(4) 7_545 13_556 ?
P6 Eu7 P6 174.972(12) 4_556 13_556 ?
P2 Eu7 P7 172.71(4) 7_545 . ?
P6 Eu7 P7 96.86(4) 4_556 . ?
P6 Eu7 P7 79.63(4) 13_556 . ?
P2 Eu7 P2 85.62(5) 7_545 . ?
P6 Eu7 P2 87.00(4) 4_556 . ?
P6 Eu7 P2 89.36(4) 13_556 . ?
P7 Eu7 P2 89.43(4) . . ?
P2 Eu7 P7 102.49(4) 7_545 13_556 ?
P6 Eu7 P7 100.43(4) 4_556 13_556 ?
P6 Eu7 P7 82.71(4) 13_556 13_556 ?
P7 Eu7 P7 81.78(5) . 13_556 ?
P2 Eu7 P7 169.07(4) . 13_556 ?
P2 Eu7 Sn2 131.91(3) 7_545 . ?
P6 Eu7 Sn2 135.78(3) 4_556 . ?
P6 Eu7 Sn2 39.86(3) 13_556 . ?
P7 Eu7 Sn2 41.56(3) . . ?
P2 Eu7 Sn2 79.88(3) . . ?
P7 Eu7 Sn2 89.22(3) 13_556 . ?
P2 Eu7 Eu3 137.20(3) 7_545 . ?
P6 Eu7 Eu3 48.98(3) 4_556 . ?
P6 Eu7 Eu3 127.78(3) 13_556 . ?
P7 Eu7 Eu3 48.20(3) . . ?
P2 Eu7 Eu3 91.88(3) . . ?
P7 Eu7 Eu3 87.11(3) 13_556 . ?
Sn2 Eu7 Eu3 89.183(13) . . ?
P2 Eu7 Eu5 49.08(3) 7_545 7_545 ?
P6 Eu7 Eu5 137.30(3) 4_556 7_545 ?
P6 Eu7 Eu5 46.06(3) 13_556 7_545 ?
P7 Eu7 Eu5 125.68(3) . 7_545 ?
P2 Eu7 Eu5 89.78(3) . 7_545 ?
P7 Eu7 Eu5 90.10(3) 13_556 7_545 ?
Sn2 Eu7 Eu5 85.043(14) . 7_545 ?
Eu3 Eu7 Eu5 173.620(10) . 7_545 ?
P2 Eu7 Eu2 129.36(3) 7_545 . ?
P6 Eu7 Eu2 89.08(3) 4_556 . ?
P6 Eu7 Eu2 85.89(3) 13_556 . ?
P7 Eu7 Eu2 45.91(3) . . ?
P2 Eu7 Eu2 43.74(3) . . ?
P7 Eu7 Eu2 127.67(3) 13_556 . ?
Sn2 Eu7 Eu2 53.013(10) . . ?
Eu3 Eu7 Eu2 61.233(9) . . ?
Eu5 Eu7 Eu2 116.669(11) 7_545 . ?
P2 Eu7 Eu5 85.67(3) 7_545 10_556 ?
P6 Eu7 Eu5 42.30(3) 4_556 10_556 ?
P6 Eu7 Eu5 133.97(3) 13_556 10_556 ?
P7 Eu7 Eu5 94.57(3) . 10_556 ?
P2 Eu7 Eu5 44.70(3) . 10_556 ?
P7 Eu7 Eu5 142.14(3) 13_556 10_556 ?
Sn2 Eu7 Eu5 112.818(13) . 10_556 ?
Eu3 Eu7 Eu5 63.988(10) . 10_556 ?
Eu5 Eu7 Eu5 120.906(14) 7_545 10_556 ?
Eu2 Eu7 Eu5 60.219(8) . 10_556 ?
P2 Eu7 Eu5 85.76(3) 7_545 . ?
P6 Eu7 Eu5 131.97(3) 4_556 . ?
P6 Eu7 Eu5 44.69(3) 13_556 . ?
P7 Eu7 Eu5 86.96(3) . . ?
P2 Eu7 Eu5 45.06(3) . . ?
P7 Eu7 Eu5 127.39(3) 13_556 . ?
Sn2 Eu7 Eu5 52.284(11) . . ?
Eu3 Eu7 Eu5 121.221(13) . . ?
Eu5 Eu7 Eu5 56.662(12) 7_545 . ?
Eu2 Eu7 Eu5 60.090(8) . . ?
Eu5 Eu7 Eu5 89.710(12) 10_556 . ?
P3 Sn1 P7 109.33(5) . . ?
P3 Sn1 P1 116.02(6) . . ?
P7 Sn1 P1 108.34(6) . . ?
P3 Sn1 Sn3 107.06(4) . 11_566 ?
P7 Sn1 Sn3 106.45(4) . 11_566 ?
P1 Sn1 Sn3 109.24(5) . 11_566 ?
P3 Sn1 Eu1 58.43(4) . . ?
P7 Sn1 Eu1 114.98(4) . . ?
P1 Sn1 Eu1 59.29(5) . . ?
Sn3 Sn1 Eu1 138.548(17) 11_566 . ?
P3 Sn1 Eu2 113.13(4) . . ?
P7 Sn1 Eu2 56.57(4) . . ?
P1 Sn1 Eu2 55.80(4) . . ?
Sn3 Sn1 Eu2 139.616(18) 11_566 . ?
Eu1 Sn1 Eu2 70.846(9) . . ?
P3 Sn1 Eu3 56.26(4) . . ?
P7 Sn1 Eu3 55.23(4) . . ?
P1 Sn1 Eu3 117.36(5) . . ?
Sn3 Sn1 Eu3 133.171(17) 11_566 . ?
Eu1 Sn1 Eu3 74.569(14) . . ?
Eu2 Sn1 Eu3 71.154(9) . . ?
P6 Sn2 P7 106.09(6) 13_556 . ?
P6 Sn2 P5 114.96(6) 13_556 . ?
P7 Sn2 P5 109.79(5) . . ?
P6 Sn2 Sn2 109.05(4) 13_556 4_566 ?
P7 Sn2 Sn2 104.32(4) . 4_566 ?
P5 Sn2 Sn2 111.94(4) . 4_566 ?
P6 Sn2 Eu2 112.59(4) 13_556 . ?
P7 Sn2 Eu2 56.41(4) . . ?
P5 Sn2 Eu2 56.08(4) . . ?
Sn2 Sn2 Eu2 137.552(15) 4_566 . ?
P6 Sn2 Eu5 56.94(4) 13_556 . ?
P7 Sn2 Eu5 114.96(4) . . ?
P5 Sn2 Eu5 59.12(4) . . ?
Sn2 Sn2 Eu5 140.49(2) 4_566 . ?
Eu2 Sn2 Eu5 73.211(11) . . ?
P6 Sn2 Eu7 54.48(4) 13_556 . ?
P7 Sn2 Eu7 54.51(4) . . ?
P5 Sn2 Eu7 114.28(4) . . ?
Sn2 Sn2 Eu7 133.464(14) 4_566 . ?
Eu2 Sn2 Eu7 70.005(14) . . ?
Eu5 Sn2 Eu7 72.330(11) . . ?
P2 Sn3 P5 118.49(5) . 10_556 ?
P2 Sn3 P4 109.25(6) . . ?
P5 Sn3 P4 105.24(6) 10_556 . ?
P2 Sn3 Sn1 106.26(4) . 11_565 ?
P5 Sn3 Sn1 111.22(4) 10_556 11_565 ?
P4 Sn3 Sn1 105.71(5) . 11_565 ?
P2 Sn3 Eu5 58.85(4) . 10_556 ?
P5 Sn3 Eu5 61.28(4) 10_556 10_556 ?
P4 Sn3 Eu5 112.82(5) . 10_556 ?
Sn1 Sn3 Eu5 141.388(18) 11_565 10_556 ?
P2 Sn3 Eu2 54.78(4) . . ?
P5 Sn3 Eu2 120.32(4) 10_556 . ?
P4 Sn3 Eu2 55.60(4) . . ?
Sn1 Sn3 Eu2 127.986(18) 11_565 . ?
Eu5 Sn3 Eu2 75.444(12) 10_556 . ?
P2 Sn3 Eu4 112.28(4) . 9_656 ?
P5 Sn3 Eu4 55.46(4) 10_556 9_656 ?
P4 Sn3 Eu4 54.68(5) . 9_656 ?
Sn1 Sn3 Eu4 140.734(18) 11_565 9_656 ?
Eu5 Sn3 Eu4 69.787(13) 10_556 9_656 ?
Eu2 Sn3 Eu4 72.733(12) . 9_656 ?
Sn1 P1 Sn1 106.18(8) . 12_655 ?
Sn1 P1 Eu2 156.73(9) . 12_655 ?
Sn1 P1 Eu2 80.15(2) 12_655 12_655 ?
Sn1 P1 Eu2 80.15(2) . . ?
Sn1 P1 Eu2 156.73(9) 12_655 . ?
Eu2 P1 Eu2 85.92(6) 12_655 . ?
Sn1 P1 Eu1 75.80(5) . . ?
Sn1 P1 Eu1 75.80(5) 12_655 . ?
Eu2 P1 Eu1 84.42(5) 12_655 . ?
Eu2 P1 Eu1 84.42(5) . . ?
Sn1 P1 Eu6 98.85(6) . . ?
Sn1 P1 Eu6 98.85(6) 12_655 . ?
Eu2 P1 Eu6 102.28(6) 12_655 . ?
Eu2 P1 Eu6 102.28(6) . . ?
Eu1 P1 Eu6 170.74(8) . . ?
Sn3 P2 Eu2 81.76(5) . . ?
Sn3 P2 Eu7 96.42(5) . 7_545 ?
Eu2 P2 Eu7 174.19(6) . 7_545 ?
Sn3 P2 Eu5 77.78(4) . 10_556 ?
Eu2 P2 Eu5 91.98(4) . 10_556 ?
Eu7 P2 Eu5 93.03(5) 7_545 10_556 ?
Sn3 P2 Eu5 103.66(5) . . ?
Eu2 P2 Eu5 91.35(5) . . ?
Eu7 P2 Eu5 83.69(4) 7_545 . ?
Eu5 P2 Eu5 176.53(6) 10_556 . ?
Sn3 P2 Eu7 163.96(7) . . ?
Eu2 P2 Eu7 88.78(5) . . ?
Eu7 P2 Eu7 94.19(4) 7_545 . ?
Eu5 P2 Eu7 89.71(4) 10_556 . ?
Eu5 P2 Eu7 89.42(4) . . ?
Sn1 P3 Eu2 162.43(7) . 4_556 ?
Sn1 P3 Eu4 95.31(5) . . ?
Eu2 P3 Eu4 93.56(5) 4_556 . ?
Sn1 P3 Eu1 78.12(4) . . ?
Eu2 P3 Eu1 86.80(4) 4_556 . ?
Eu4 P3 Eu1 89.73(4) . . ?
Sn1 P3 Eu3 82.01(5) . . ?
Eu2 P3 Eu3 89.17(4) 4_556 . ?
Eu4 P3 Eu3 177.26(6) . . ?
Eu1 P3 Eu3 90.30(4) . . ?
Sn1 P3 Eu5 103.48(5) . 11_566 ?
Eu2 P3 Eu5 92.16(4) 4_556 11_566 ?
Eu4 P3 Eu5 86.54(4) . 11_566 ?
Eu1 P3 Eu5 176.06(6) . 11_566 ?
Eu3 P3 Eu5 93.48(5) . 11_566 ?
Sn3 P4 Sn3 112.26(9) . 12_655 ?
Sn3 P4 Eu2 165.92(8) . 12_655 ?
Sn3 P4 Eu2 79.82(2) 12_655 12_655 ?
Sn3 P4 Eu2 79.81(2) . . ?
Sn3 P4 Eu2 165.93(8) 12_655 . ?
Eu2 P4 Eu2 87.35(6) 12_655 . ?
Sn3 P4 Eu4 83.29(6) . 9_656 ?
Sn3 P4 Eu4 83.29(6) 12_655 9_656 ?
Eu2 P4 Eu4 91.30(6) 12_655 9_656 ?
Eu2 P4 Eu4 91.30(6) . 9_656 ?
Sn3 P4 Eu4 95.96(6) . 2_654 ?
Sn3 P4 Eu4 95.96(6) 12_655 2_654 ?
Eu2 P4 Eu4 89.69(5) 12_655 2_654 ?
Eu2 P4 Eu4 89.69(5) . 2_654 ?
Eu4 P4 Eu4 178.63(8) 9_656 2_654 ?
Sn3 P5 Sn2 101.91(6) 10_566 . ?
Sn3 P5 Eu2 161.57(7) 10_566 . ?
Sn2 P5 Eu2 80.09(4) . . ?
Sn3 P5 Eu4 82.87(5) 10_566 2_654 ?
Sn2 P5 Eu4 157.84(7) . 2_654 ?
Eu2 P5 Eu4 88.76(4) . 2_654 ?
Sn3 P5 Eu6 97.96(5) 10_566 . ?
Sn2 P5 Eu6 95.06(5) . . ?
Eu2 P5 Eu6 100.12(5) . . ?
Eu4 P5 Eu6 105.79(5) 2_654 . ?
Sn3 P5 Eu5 74.93(4) 10_566 . ?
Sn2 P5 Eu5 77.93(4) . . ?
Eu2 P5 Eu5 87.75(4) . . ?
Eu4 P5 Eu5 82.57(4) 2_654 . ?
Eu6 P5 Eu5 168.51(6) . . ?
Sn2 P6 Eu5 162.50(7) 13_556 11_566 ?
Sn2 P6 Eu3 100.04(5) 13_556 . ?
Eu5 P6 Eu3 95.66(5) 11_566 . ?
Sn2 P6 Eu5 81.64(5) 13_556 13_556 ?
Eu5 P6 Eu5 83.69(4) 11_566 13_556 ?
Eu3 P6 Eu5 173.05(6) . 13_556 ?
Sn2 P6 Eu7 96.96(5) 13_556 4_556 ?
Eu5 P6 Eu7 92.91(5) 11_566 4_556 ?
Eu3 P6 Eu7 81.59(4) . 4_556 ?
Eu5 P6 Eu7 91.53(4) 13_556 4_556 ?
Sn2 P6 Eu7 85.65(5) 13_556 13_556 ?
Eu5 P6 Eu7 84.98(4) 11_566 13_556 ?
Eu3 P6 Eu7 96.36(5) . 13_556 ?
Eu5 P6 Eu7 90.48(4) 13_556 13_556 ?
Eu7 P6 Eu7 176.91(6) 4_556 13_556 ?
Sn2 P7 Sn1 109.20(6) . . ?
Sn2 P7 Eu3 161.77(7) . . ?
Sn1 P7 Eu3 81.48(4) . . ?
Sn2 P7 Eu2 79.98(4) . . ?
Sn1 P7 Eu2 79.71(5) . . ?
Eu3 P7 Eu2 87.76(4) . . ?
Sn2 P7 Eu7 83.93(5) . . ?
Sn1 P7 Eu7 159.30(7) . . ?
Eu3 P7 Eu7 82.04(4) . . ?
Eu2 P7 Eu7 87.23(4) . . ?
Sn2 P7 Eu7 98.92(5) . 13_556 ?
Sn1 P7 Eu7 95.49(5) . 13_556 ?
Eu3 P7 Eu7 94.55(4) . 13_556 ?
Eu2 P7 Eu7 174.32(6) . 13_556 ?
Eu7 P7 Eu7 98.22(5) . 13_556 ?

_refine_diff_density_max         2.081
_refine_diff_density_min         -2.631
_refine_diff_density_rms         0.480

_shelxl_version_number           2013-4

